Presentation on theme: "Construction Materials (CE 1206)"— Presentation transcript:
1 Construction Materials (CE 1206) BITUMINOUS MATERIAL
2 BackgroundAsphalt cement and tar are considered bituminous materials. Quite often, these two terms are used interchangeably due to misconception resulting from their similarity in appearance.Asphalt cement and tar are two distinctly different materials with different origins and different chemical and physical characteristic.
3 Cont..Asphalt cement is a dark brown to black cementitious materials either its naturally occurred or produced by petroleum distillation.Tar however, is primarily manufactured from the destructive distillation of bituminous coal and has a very distinct ordor.Tar is hardly used in paving. Why?Some undesirable physical characteristic such as very high temperature susceptibility.Significant health hazards such as severe eye and skin irritation when exposed to its fume.
4 Cont.. Asphalt can be classified into two categories: Natural asphalt Petroleum asphaltNatural asphalt – laid down in geologic strata and occur relatively as soft asphalt material and also as a hard, friable, black material in veins of rock formation. Hundred of thousands of tons of asphalt have been removed from the Trinidad Lake without it showing any appreciable sign of loss.
5 Cont..Petroleum asphalt – these are colloidally dispersed hydrocarbons in crude petroleum and are obtained by refining petroleum crudes. Gradually, these refined asphalt became plentiful and good quality. This forced the natural asphalt into position of relative unimportance.
6 Asphalt: Types and Uses Asphalt commonly used in flexible pavement construction and can be divided into three (3) types:Asphalt cementEmulsified asphaltCutback asphalt
7 Asphalt CementsAs discussed earlier, asphalt cement obtained by distillation process from crude petroleum using different refining process.Ambient temperature – asphalt cement is black, sticky and semisolid and highly viscous material. Its also strong and durable with excellent adhesive and water proofing characteristic, highly resistant to the action of most acids, alkalies and salt.
8 Cont.. How do we grade asphalt cement? Two method: based on penetration and viscosity.Penetration: As specified in ASTM D946, there are five (5) standard penetration graded of asphalt cement, , 60-70, , and The penetration grade is based from the penetration test.Penetration test involve measurements of penetration of standard penetration needle into a sample of asphalt cement under standard temperature, time and load.
9 Cont..Viscosity: As specified in ASTM D3381, this grading is based on the viscosity test. The viscosity grading system is based from original asphalt cement include AC-2.5, AC-5, AC-10, AC-20, AC-30 and AC-40.
10 Emulsified AsphaltEmulsified asphalt (emulsion) is a mixture of asphalt cement, water and emulsified agent. This emulsified asphalt is usually used for prime coat (binder and road-base) and tack coat (binder and wearing).Because the asphalt cement will not dissolve in water, asphalt cement and water exist in separate phases as in figure shown.
12 Cutback AsphaltCutback asphalts are liquid asphalts which are manufactured by adding (cutting back) petroleum solvents to asphalt cements.They are made to reduce the asphalt viscosity for lower application temperature. Application to aggregate or pavement causes the solvent to escape by evaporation and leave the asphalt cement residue on the surface.Based on the rate of evaporation, cutback asphalt are divided to three types – rapid curing (RC), medium curing (MC) and slow curing (SC).
13 Cont..RC – produce by adding a light diluent of high volatility (gasoline or naphtha) to asphalt cement. These are used primarily for tack coat and surface treatment.MC – produce by adding a medium diluent of intermediate volatility (kerosene) to asphalt cement. These are generally used for prime coat and road mixing operation.SC – produce by adding oils of low volatility (diesel or other gas oil) to asphalt cement. They are generally used for prime coat and dust palliatives.
14 The depth of penetration is measured in unit of 0 The depth of penetration is measured in unit of 0.1 mm and is reported as penetration units (ie. Needle penetrate 8mm, the penetration of asphalt is 80).
15 A steel ball of specified dimensions and weight is placed in the center of the sample. The bath is heated at a controlled rate of 5oC per minute.When the asphalt soften, the ball and the asphalt will sink to the bottom of the beaker. The temperature is recorded the minute when the soften asphalt sink the prescribes distances and touch the bottom plate.
19 Asphalt Mix Types Stone Mastic Asphalt gap graded impermeable large stone to stone contacthigh in binder contentuses bitumen Penetration Gradewithstand higher loading and trafficimprove rut resistance and pavement durability
Your consent to our cookies if you continue to use this website.